Presentation on theme: "Pre-Filming Method of Reducing Metal Release from Alloy 690 for SG in Primary Water of PWR 2009 ISOE Asian ALARA Symposium Aomori September 9, 2009 Sumitomo."— Presentation transcript:
Pre-Filming Method of Reducing Metal Release from Alloy 690 for SG in Primary Water of PWR 2009 ISOE Asian ALARA Symposium Aomori September 9, 2009 Sumitomo Metal Industries, Ltd. Akihiro Uehira Manabu Kanzaki Kazuyuki Kitamura Hiroyuki Anada September 2009 1
Contents 1)Background 2) Selective oxidation of Cr oxide for pre-filming and characterization 3)Ni release of pre-filmed alloy 690 4) Conclusion September 2009 2
Background 1) Radioactive resources are mainly released metal, Co and Ni etc. from primary water structures in PWR. 2) Especially, area of SG (Steam Generator) tubes contacting with the primary water is the largest among those of primary water structures. 3) Therefore, reduction of metal release from SG tubes is the most effective in order to reduce exposure. September 2009 3
Ni Release from SG Tubes Reactor Core 58 Ni 58 Co Ni releases from SG tube to primary water. 58 Ni Primary water Steam Generator (SG) (Alloy 690 ： 60Ni-30Cr-9Fe) SG tube Release Adhere to primary circuit structures. 1)Radioactive nuclide that governs radiation effect is mainly 58 Co which comes from Ni base alloy used as SG tube. 2)It is important to study the method of reducing metal release from SG tube from the viewpoint of reducing exposure. Move to reactor core. Nuclear fuelPrimary water Ni is transformed to radioactive Co. Figure 1 September 2009 4 n(Neutron) 58 Ni
Figure 2 Image of Ni Release from SG Tubes during Operation Cycle Main Ni release from SG tubes occurs in the early operation period. In order to reduce total Ni release, reduction of Ni release in the early operation period is the most effective. Ni Release from SG Tubes Operation Cycle Ni Release from SG Tubes during Operation Cycle Ni release is decreasing during the early operation period because the barrier generates on the surface of SG tubes. Main Ni Release September 2009 5
Figure 3 Image of Ni Release Reduction Pre-filming on the SG tube surface is expected to reduce Ni release in the early operation period. Ni Release Operation Cycle Reduction of Ni Release by Pre-Filming on SG Tubes Surface SG tube Pre-filmed barrier Prevent Ni migration. 58 Ni Primary water Ni release reduction by pre-filming September 2009 6
Co release in Higashidori Nuclear Power Station, BWR, decreased by pre-filming on the surface of feed water heater tube, about 1/2 compared with other plant without pre-filming method. (*)Sato, Tohoku Electric Power Company, The thermal and nuclear power generation convention 2008 Sendai Commercial Application of Pre-Filming Method Co Ion Concentration [ppb] EFPH (Equivalent Full Power Hours) Figure 4 Process of Co Ion Concentration in Nuclear Reactor Water Higashidori applying pre-filming method September 2009 7 Co concentration decreased.
( L. Guinard, EDF, Water Chemistry of Nuclear Reactor Systems 8, BNES, 2000) R&D of Pre-Filming Method to Alloy 690 Released metal weight (mg/dm 2 ) September 2009 8 As different pre-filming method from below methods, we researched oxidation at high temperature. Figure 5 Quantity of Released Metal during the Corrosion Test
Cr oxide is stable in primary water of PWR. We considered that Cr oxide film is suitable as a barrier against Ni release from SG tubes to primary water during operation. Stable region of Cr 2 O 3 Primary water in PWR Figure 6 Potential-pH Diagram of Cr in 300 ℃ Water Potential (Volts vs SHE) pH September 2009 9 Possibility of Cr Oxide as Pre-Film Candidate
Alloy 690 contains 30% Cr. We considered that Cr oxide can be formed on the surface of alloy 690 by control of oxygen potential and temperature. Cr Oxide on alloy 690 4/3Cr+O 2 =2/3Cr 2 O 3 2Ni+O 2 =2NiO 2Fe+O 2 =2FeO Figure 7 Relationship between Type of Oxide and Oxidation Condition Temperature Partial Pressure of Oxygen September 2009 10 Cr is oxidized selectively in this region.
1) Clarify the possibility of selective oxidation of Cr in alloy 690 by controlling oxygen partial pressure and temperature. 2) Clarify the effectiveness of pre-filming on Ni release reduction from alloy 690. Objective September 2009 11
Specimen : Alloy 690 sheet (60Ni-30Cr-10Fe) Heat treatment →Cold rolling →Sampling test specimen →Surface polishing →Pre-filming Preparation of Test Specimen September 2009 12
Pre-Filming Method H 2 O in H 2 Gas Quartz vessel Electric furnace Test specimen Figure 8 Pre-Filming Equipment September 2009 13 1)Oxide film formation by oxygen at high temperature. 2) H 2 O in H 2 gas as oxygen source.
Appearance of Oxide Film After pre-filming Bare specimen (Before pre-filming) Photo 1 Appearance of Specimen September 2009 14
Cross Section of Oxide Film Oxide film Homogenous oxide film was formed on the surface of the specimen. Specimen (Alloy 690) Photo 2 Crosse Section of Oxide Film (SEM) September 2009 15 1 μm
Oxide film is mainly composed of Cr 2 O 3. Depth from Surface (nm) Relative Oxygen Intensity Proportion (%) of Constituent Metal Element Thickness of oxide film Composition of Oxide Film Ni CrO Mn Fe 120000 100000 8000 0 6000 0 4000 0 2000 0 0 100 80 60 40 20 0 05001000150020002500 Specimen Cr 2 O 3 MnCr 2 O 4 September 2009 16 Figure 9 Analysis of oxide film by SIMS
Ni Release Test on Various Thickness Oxide Film September 2009 17
Ni Release Test Method Test specimen Platinum container Electric furnace Deionized water After immersion in deionized water at 320 ℃ for 1000 hrs, Ni content in deionized water was measured by ICP. Figure 10 Ni Release Test Equipment September 2009 18
Ni Release Test Result of Pre-Filmed Specimen Ni release decreased from 0.9 ppm to 0.01 ppm by pre-filming, regardless of oxide film thickness. Figure 11 Effect of Oxide Film on Reduction of Ni Release Ni release decreased Drastically by pre-filming. September 2009 19
Following results were obtained. 1) Cr oxide film can be formed on the surface of alloy 690 by using H 2 O in H 2 gas at high temperature. 2) The oxide film is mainly composed of Cr 2 O 3. 3)Pre-filming of Cr 2 O 3 decreased Ni release from alloy 690 by a factor of 0.1. 4) Ni release from SG tubes in PWR can be expected to reduce by this pre-filming. Conclusion September 2009 20
Thank you for your attention. September 2009 21